Anti-Icing Superhydrophobic jwu/papers/la902882b_anti-Icing.pdf Anti-Icing Superhydrophobic...
Embed Size (px)
Transcript of Anti-Icing Superhydrophobic jwu/papers/la902882b_anti-Icing.pdf Anti-Icing Superhydrophobic...
12444 DOI: 10.1021/la902882b Langmuir 2009, 25(21), 1244412448Published on Web 10/05/2009
2009 American Chemical Society
Anti-Icing Superhydrophobic Coatings
Liangliang Cao, Andrew K. Jones, Vinod K. Sikka, Jianzhong Wu, and Di Gao*,
Department of Chemical and Petroleum Engineering, University of Pittsburgh, Pittsburgh, Pennsylvania 15261,Ross Technology Corporation, Leola, Pennsylvania 17540, and Department of Chemical and Environmental
Engineering, University of California, Riverside, California 92521
Received August 4, 2009. Revised Manuscript Received September 26, 2009
We use nanoparticle-polymer composites to demonstrate the anti-icing capability of superhydrophobic surfaces andreport direct experimental evidence that such surfaces are able to prevent ice formation upon impact of supercooledwater both in laboratory conditions and in natural environments. We find that the anti-icing capability of thesecomposites depends not only on their superhydrophobicity but also on the size of the particles exposed on the surface.The critical particle sizes that determine the superhydrophobicity and the anti-icing property are in two different lengthscales. The effect of particle size on ice formation is explained by using a classical heterogeneous nucleation theory. Thisresult implies that the anti-icing property of a surface is not directly correlated with the superhydrophobicity, and thus, itis uncertain whether a superhydrophobic surface is anti-icing without detailed knowledge of the surface morphology.The result also opens up possibilities for rational design of anti-icing superhydrophobic surfaces by tuning surfacetextures in multiple length scales.
Inspired by the self-cleaning properties of lotus leaves,1,2
researchers have recently made significant progress in fabricationof superhydrophobic surfaces,3-10 on which water droplets beadup with a contact angle greater than 150 and drip off rapidlywhen the surface is slightly inclined. The superhydrophobicity,characterized by the high contact angle and small hysteresis ofwater droplets, on such surfaces has been attributed to a layer ofair pockets formed between water and a rough substrate.11-13
One attractive application of superhydrophobic surfaces, inaddition to the extraordinary water-repellency, is their speculatedcapability to reduce accumulation of snow and ice and to evencompletely prevent formation of ice on solid surfaces.14-16
Several groups have studied the adhesion of ice on superhydro-phobic surfaces and have found correlations, with a reasonabledegree of success, between reduction in ice adhesion and thesuperhydrophobicity of surfaces.14-16 However, we are unawareof published research to study ice formation on superhydrophobicsurfaces.
Among numerous problems caused by icing, many are due tostriking of supercooled water droplets onto a solid surface. Such
icing caused by supercooled water, also known as freezing rain,atmospheric icing, or impact ice, is notorious for glazingroadways, breaking tree limbs and power lines, and stalling airfoilof aircrafts, which may cause immeasurable economic losses.17,18
Whereas extensive work has been published on superhydropho-bicity, up to date there is little experimental/theoretical work onice formation from supercooled water on superhydrophobicsurfaces. The speculation on the anti-icing property of super-hydrophobic surfaces, especiallywhen supercooledwater dropletsstrike such surfaces, has been under debate for many years.
In this work, we study the anti-icing property of superhydro-phobic coatings prepared by using nanoparticle-polymer com-posites.Wedemonstrate thatwhen the size of the particles in thesecomposites is in the right range, the coatings are able to prevent iceformation upon impact of supercooled water both in laboratoryconditions and in naturally occurring environments.More impor-tantly, we find that the anti-icing capability of these compositesdepends not only on their superhydrophobicity but also on thesize of the particles exposed on the surface. The critical particlesizes that determine the superhydrophobicity and the anti-icingproperty are in two different length scales. These results open uppossibilities for rational design of anti-icing superhydrophobicsurfaces by tuning surface textures in multiple length scales.
Synthesis of Acrylic PolymerResin. In a typical process, theacrylic polymer was synthesized by free radical polymerization ofstyrene, butyl methacrylate, and glycidyl methacrylate in tolueneusing azodiisobutyronitrile (AIBN) as the initiator. All thesechemicals were purchased from Sigma-Aldrich. In a three-neckedround-bottomed flask equipped with a magnetic stirrer, a con-denser, a funnel, and a thermometer, 3 g of styrene, 15 g of butylmethacrylate, 4 g of glycidyl methacrylate, and 100mL of tolueneweremixed.Themixturewas stirred andheated to 85 C.The heat
*Corresponding author. E-mail: email@example.com. Telephone: 412-624-8488. Fax: 412-624-9639.(1) Barthlott, W.; Neinhuis, C. Planta 1997, 202, 18.(2) Neinhuis, C.; Barthlott, W. Ann. Bot. 1997, 79, 667667.(3) Blossey, R. Nat. Mater. 2003, 2, 301306.(4) Erbil, H.Y.; Demirel, A. L.; Avci, Y.;Mert, O.Science 2003, 299, 13771380.(5) Onda, T.; Shibuichi, S.; Sotah, N.; Tsujii, K. Langmuir 1996, 12, 21252127.(6) Sun, T. L.; Feng, L.; Gao, X. F.; Jiang, L.Acc. Chem. Res. 2005, 38, 644652.(7) Gao, L. C.; McCarthy, T. J. J. Am. Chem. Soc. 2006, 128, 90529053.(8) Tuteja, A.; Choi, W.; Ma, M. L.; Mabry, J. M.; Mazzella, S. A.; Rutledge,
G. C.; McKinley, G. H.; Cohen, R. E. Science 2007, 318, 16181622.(9) Xiu, Y. H.; Zhu, L. B.; Hess, D. W.; Wong, C. P. Nano Lett. 2007, 7, 3388
3393.(10) Nakajima, A.; Hashimoto,K.;Watanabe, T.Monatsh. Chem. 2001, 32, 3141.(11) Cassie, A. B. D.; Baxter, S. Trans. Faraday Soc. 1944, 40, 546551.(12) Herminghaus, S. Europhys. Lett. 2000, 52, 165170.(13) Lafuma, A.; Quere, D. Nat. Mater. 2003, 2, 457460.(14) Saito, H.; Takai, K.; Yamauchi, G. Surf. Coat. Int. 1997, 80, 168171.(15) Nakajima, A.; Hashimoto, K.; Watanabe, T. Monatsh. Chem. 2001, 132,
3141.(16) Kulinich, S. A.; Farzaneh, M. Appl. Surf. Sci. 2009, 255, 81538157.
(17) Cober, S. G.; Isaac, G. A.; Strapp, J. W. J. Appl. Meteorol. 2001, 40, 19842002.
(18) Lasher-Trapp, S.; Anderson-Bereznicki, S.; Shackelford, A.; Twohy, C. H.;Hudson, J. G. J. Clim. Appl. Meteorol. 2008, 47, 26592678.
DOI: 10.1021/la902882b 12445Langmuir 2009, 25(21), 1244412448
Cao et al. Letter
source was then turned off. A solution of 0.2 g ofAIBN in 2.5mLof toluene was dropwise added into the flask. The reactionmixture was heated to 85 C and stirred isothermally for 3 h.Afterward, the same amount of AIBN/toluene solution wasadded into the flask, and the mixture was stirred for another3 h. At the end of the reaction, the mixture was cooled at roomtemperature. The resulting acrylic polymer was precipitated inhexane, filtered, and then dried under vacuum at 40 C for 24 h.The molecular weight of the polymer was determined by gelpermeation chromatography (Shimadzu). The number averagemolecular weight of the polymer was about 18000 g/mol, and theweight average molecular weight was about 48000 g/mol.
Preparation of the Polymer Binder. In a typical process, thepolymer binder was prepared by mixing 2 g of the synthesizedacrylic polymer, 1 g of silicone resin (DOW CORNING 840RESIN, 60 wt% in toluene), 1 g of toluene, and 0.6 g of acetone.The binder can be cured either at room temperature for 12 h or at80 C for 2 h. During the curing process, the reactive glycidylgroups on the acrylic polymers cross-link with the silicone resin.The static water contact angle of the cured binder is 107.Preparation of the Particle-Polymer Composites. The
particle-polymer composites were prepared by mixing about2.5 g of the organosilane-modified silica particles of variousdiameters (20 nm, 50 nm, 100 nm, 1 m, 10 m, and 20 m) with5 g of the polymer binder, 75 g of toluene, and 15 g of acetone.They were applied on Al plates by using a spray gun at a pressureof about 30 psi and cured at room temperature for 12 h.
Electron Microscopy. Scanning electron microscopy (SEM)images and energy dispersive X-ray spectra were taken on aPhilips XL-30 field emission SEM setup. A thin palladium/goldfilm was sputtered on the sample before SEM images were taken.Transmission electron microscopy images were taken using aJEOL 200CX microscope.
Contact AngleMeasurement. Thewater contact anglesweremeasured by using a VCA-OPTIMA drop shape analysis system(AST Products, Inc.) with a computer-controlled liquid dispen-sing system and a motorized tilting stage. Water droplets with avolume of 4 L were used to measure the static water contactangle. The advancing and receding angles were recorded duringexpansion and contraction of the droplets induced by placing aneedle in the water droplets and continuously supplying andwithdrawing water through the needle. The sliding angle wasmeasuredby tilting the stage and recordedwhen thedroplet beganto move in the downhill direction. Each measurement wasrepeated three times. The measurement was performed undernormal laboratory ambient conditions (20 C and 30% relativehumidity). The intrinsic water contact angle on the silica particleswas estimated bymeasuring thewater contact angle on a flat silicasurface modified with the same surface chemistry.
Icing Experiments Using Laboratory-made SupercooledWater. Supercooled water was prepared by storing bottled purewater in a -20 C freezer for 3 h. The coated and uncoated Alplates were also stored in the -20 C freezer for 3 h before theexperiments and were tilted at an angle of about 10 to thehorizontal plane during the experiments. A volume of 500 mLof supercooled water was poured onto the